(2) PHYSICAL REVIEW B 80, 085107 共2009兲. LÓPEZ et al.. it has been also studied by using density-functional theory 共DFT兲 in the framework of the conjugate-gradient iterative minimization technique.10 Structure optimization from two different initial configurations gave rise to structures both of them characterized for having an Fe central atom with the others forming a cage with an Fe-O interatomic distance between the central atom and an oxygen in the surroundings surprisingly large, i.e., 3.087 Å and 3.141 Å in the two cases. Magnetic and vibrational calculations of this magic cluster have been also performed on the basis of an allelectron DFT.11 Results revealed a structure characterized also by a central Fe atom and a distance Fe-O relative to the central atom of 3.31 Å and a total moment of 32B when considering a ferromagnetic state. If ferrimagnetic coupling is considered, clusters are characterized by an Fe-O distance relative to the central atom of 3.23 Å and a total moment of 14B. Other magic transition-metal oxide clusters have been also reported to occur.12 On the other hand, as is well established, the magnetic and electronic properties are strongly dependent on the specific atomic surface reconstruction as it has been studied in iron oxides such as magnetite by using DFT with the GGA + U and LDA+ U approaches.13 Thus, the fact of being able to tailor the properties of small clusters by changing size and composition like the proportion of Fe and O atoms, as concerns to FenOm clusters, has motivated us to consider this kind of clusters. The purpose of this article is to characterize from different perspectives 共electronic, magnetic, and structural兲 iron oxide clusters of the form FenOm when these are constructed on the basis of a well-studied iron oxide such as magnetite 共Fe3O4兲 and starting from the two different space groups ascribed to this material, namely cubic 共Fd3̄m兲 and monoclinic 共P2 / c兲, which correspond to the structures of bulk magnetite above and below the Verwey temperature, respectively.14,15 In this work we report on FenOm clusters having 33, 45, and 113 atoms corresponding to the following stoichiometries Fe17O16, Fe17O28, and Fe45O68. Finally, we want to stress that to the best of our knowledge, no firstprinciples studies on FenOm clusters having several tens of atoms have yet been reported. II. COMPUTATIONAL DETAILS. Electronic structure and density of state 共DOS兲 calculations were performed using DFT 共Ref. 16兲 in the framework of the GGA+ U approach on the basis of the Dudarev’s method17 and using the PW91 pseudopotential for the exchange-correlation functional with the Vosko-Wilk-Nusair correction.18 Calculations were also performed in the framework of the projector augmented wave method19,20 as implemented in the VASP package.21 The on-site Coulomb term has been included according to the degree of localization of the Fe d electrons. We set the U parameter to 4.5 eV for Fe cations, which is based on constrained calculations.15,22–24 On this last respect, we want to stress that LDA+ U band structure calculations with U varying from 4 to 6 eV provide optical, magneto-optical and x-ray magnetic circular dichroism spectra in reasonable agreement with experimental data.23 The Hund’s coupling for Fe was set to. J = 0.89 eV.15,25 Both, the U and J parameters for oxygen were set to zero. In any case, we should stress that there is a delicate balance between U and J which in principle can lead to differences regarding the final magnetic state of the system. Therefore, we have decided to choose the parameters already used and reported in the literature, where good agreement of a large diversity of properties have been reported. Clusters were simulated by periodic cells separated by a sufficiently high amount of vacuum in order to avoid intercluster interactions. Hence, our simulated system can be considered as a periodic and monodisperse array of isolated clusters. Two different initial crystalline structures, namely Fd3̄m and P2 / c and three different cluster sizes having 33, 45, and 113 atoms were considered corresponding to Fe17O16, Fe17O28, and Fe45O68 clusters. Hereafter, such clusters are labeled in generic form as C33, C45, and C113; and as C33F, C33P, C45F, C45P, C113F, and C113P, where F and P stand for the initial Fd3̄m and P2 / c symmetries, respectively. These amounts yield the following average diameters in the relaxed structures: 7.0共1兲, 8.2共1兲 and 12.3共1兲 Å. The lateral parameter of the supercell was set to 18 Å, 20 Å, and 24 Å for C33, C45, and C113 clusters, respectively. A Wigner-Seitz radius rWS = 1.302 Å for iron and rWS = 0.82 Å for oxygen were used. The energy cutoff for the plane wave representation was 500 eV. The convergence force criterion was set to 0.01 eV/ Å per atom. The charge of each atom was estimated by using the Bader method, where a fair partition of the electronic charge is performed by only including the valence electrons. Details of the implementation and the meaning can be found in Henkelman et al.26 This method has been used to calculate the partial charges in H and O atoms on the H2O molecule, and in crystals such as NaCl and MgO,26 where an interpretation of the electronic charge transfer has been discussed. The magnetic moment distribution was computed by integrating the electronic density within the Wigner-Seitz radius for each atom. The overall magnetization WS per cluster were also determined by summing the respective quantities per atom. Cohesive energy per one formula unit was also computed according to Ecoh = Etot − nEFe − mEO where n and m correspond to the number of Fe and O atoms with energies in the isolated state EFe and EO, respectively. Only for comparison purposes, the structural and electronic properties of bulk magnetite, taken as reference material, have also been computed. In this case, a 6 ⫻ 6 ⫻ 6 Monkhorst-Pack27 grid and a total number of 28 k points in the irreducible Brillouin zone were employed for the Fd3̄m symmetry, whereas a 6 ⫻ 6 ⫻ 2 Monkhorst-Pack grid with 36 k points for P2 / c symmetry was considered. A Gaussian smearing factor of 0.01 for clusters and monoclinic bulk was employed, whereas the Methfessel-Paxton method was used for the cubic bulk.28 For clusters, calculations were done at the ⌫ point. Finally, in order to perform a structural analysis before and after the optimization process, both the radial 关RDF or g共r兲dr兴 and angular 关ADF or h共兲d兴 distribution functions were computed. To compute RDF, a cut-off distance rc approximately equals to the cluster diameter was considered. This function accounts for the number of neighbors surrounding every atom at a given distance between r and r + dr, where 0 ⱕ r ⱕ rc. To compute ADF, angles formed. 085107-2.
(3) PHYSICAL REVIEW B 80, 085107 共2009兲. STRUCTURE AND ELECTRONIC PROPERTIES OF IRON… TABLE I. Ground-state lattice and electronic properties for the cubic Fd3̄m and monoclinic P2 / c structures of bulk magnetite. Average magnetization per one formula unit 共mav兲 are given in B. Lattice constants 共a , b , c兲 are in Å, cohesive energy 共Ecoh兲 per formula unit and gap 共⌬g兲 in eV. Phase. Quantity. This work. Piekarza. Exp.. Fd3̄m. a Ecoh mav ⌬g a b c ␤ Ecoh ⌬g. 8.456 −35.791 3.825 0 6.013 6.017 16.865 90.230 −36.115 0.25. 8.446. 8.394b. 3.96 0 5.967 5.995 17.034 90.417. 4.05c 0 5.944b 5.925b 16.775b 90.237b. 0.33. 0.14d. P2 / c. a. Reference. 14. .. c. Reference 30. Reference 31.. d. by triads of atoms within spheres of 2.2 Å were considered. Finally, we have calculated a mean coordination number according to the following proposed relationship N. Space group Fd3̄m. bReference 29.. N. r 1 具z共r兲典 = 兺 兺 ␦共ri − r j兲, Nr ri苸关r,r+dr兴 j=1. TABLE II. Valence electric charge 共Q兲 in e units and magnetic moments per atom 共兲 in B, for the cubic Fd3̄m, and monoclinic P2 / c structures of bulk magnetite.. 共1兲. where N is the total number of atoms and Nr is the number of atoms at a distance ri belonging to the interval 关r , r + dr兴. This mean value was computed by considering the total number of neighbors per atom within the entire cluster. Histograms showing the way as the atoms become spatially distributed were also computed. These quantities allows having a full structural characterization of the clusters. III. RESULTS AND DISCUSSION. In Table I we show the ground-state lattice and electronic properties for Fd3̄m and P2 / c structures of bulk magnetite, our reference material, obtained in the present calculations. Experimental data and theoretical results by Piekarz et al.14 are also listed for comparison. Results show an overall good agreement with experimental data of Refs. 29–31 and with those of Piekarz et al.,14 wherever available. It must also be noticed that the ground-state cohesive energy of the crystal Ecoh per one formula unit is much smaller in the P2 / c phase than in the Fd3̄m phase, indicating that the low temperature monoclinic phase of P2 / c symmetry is the most stable. This fact agrees with several results in the literature where the monoclinic phase has been reported as the lowest-energy state.14,15,29 Data corresponding to charge and magnetization per atom for both phases are listed in Table II. In the case of the cubic phase, different labels 共B1, B2, B3兲 have been employed to compare the parameters associated to iron cat-. P2 / c. Index. Atom. Q共e兲. 共 B兲. 1,2 3,5 4 6 1,2,6,8 3–5,7 9,16,21 10,15,18,20,23 11,14,17 12,13,19,22,24. FeA Fe共B1兲 Fe共B2兲 Fe共B3兲 FeA FeA FeB FeB FeB FeB. 1.49⫾ 0.01 1.50⫾ 0.02 1.47 1.51 1.19⫾ 0.05 1.46⫾ 0.04 1.65⫾ 0.03 1.56⫾ 0.01 1.94⫾ 0.03 1.85⫾ 0.03. −4.02 3.92 4.02 3.83 −4.02 −4.02 3.65⫾ 0.01 3.66⫾ 0.01 4.12⫾ 0.01 4.12. ions in octahedral sites under bulk conditions with those corresponding to clusters. Charge and moment distribution reveal therefore the occurrence of three different octahedral Fe sites for the Fd3̄m space group, whereas two different tetrahedral Fe sites and four nonequivalent B-Fe sites are found for the P2 / c symmetry. We find these last numbers in accord with previous results where two distinct A-Fe sites and four independent octahedral B-site iron atoms were concluded from structural refinement of stoichiometric single crystals of magnetite using high-resolution x-ray and neutron powder diffraction.29 Regarding the magnetic structure for the P2 / c symmetry, while the total moment per one formula unit remains at ⬃4B the iron magnetic moments amount to −4.02B for A sites and between 3.65B and 4.13B for B sites. It must be stressed however that the magnetic moment is not a well-defined quantity in non absolute ionic crystalline systems as far as it can be partitioned depending on the chosen value for rWS. By using our value of 1.302 Å we find numerical results in rather good agreement with some others found in literature.14,15,32–35 However, it is interesting to point out that, in particular, the corresponding values for an A-Fe site are very different from the value of 5B derived from Hund’s rules and the nominal Fe3+ charge on a typical A site. This fact is consistent with the itinerant nature of magnetism in this system and with changes in the valence states. Differences in sign are consistent with an antiparallel alignment between A and B sublattices in agreement with a ferrimagnetic state. Concerning clusters, Table III shows the results corresponding to the cohesive energy and the magnetization WS. By comparing the corresponding energy values we can conclude that the ground-state phase is that resulting from the initial P2 / c symmetry. As we will show later by comparing the radial and angular distribution functions before an after relaxation, the largest C113 cluster tends to preserve the starting configuration suggesting that the monoclinic phase is energetically more stable than the cubic phase in the low temperature regime. This result in addition to the fact that such cluster, namely Fe45O68 whose chemical formula can be written also as Fe2.647O4, is stoichiometrically similar to bulk. 085107-3.
(4) PHYSICAL REVIEW B 80, 085107 共2009兲. LÓPEZ et al. TABLE III. Global parameters derived from the present calculations for the relaxed C33, C45, and C113 magnetite clusters obtained from the initial Fd3̄m and P2 / c structures.. Phase. Cluster. Ecoh 共eV兲. WS 共 B兲. Fd3̄m. 33 45 113 33 45 113. −18.933 −25.892 −31.260 −18.947 −25.958 −31.454. 32.930 28.905 43.099 27.178 28.767 43.182. P2 / c. magnetite 共Fe3O4兲, allows to suggest that magnetite nanoparticles should, in principle, exhibit Verwey transition. Such conclusion is also endorsed by the fact that the Verwey transition has also been observed in highly nonstoichiometric magnetite of the form Fe3−␦O4.36 In clusters with P2 / c symmetry, the total magnetization increases as the cluster size is increased. However, this is not strictly the case for clusters with Fd3̄m symmetry where the total magnetization of the smallest cluster 共C33兲, is greater than that of C45. This fact is due to a parallel alignment of one of the A spins respect to the B spins 共see Table IV兲 giving rise to a ferromagnetic state. Figures 1 and 2 show the resulting atomic and charge distribution for the relaxed clusters starting from symmetries Fd3̄m and P2 / c, respectively. Results corresponding to charge and magnetic moment per atom are listed in Tables IV and V for C33F and C33P respectively, whereas those for C45F and C45P are listed in Tables VI and VII, respectively. From these results several features are remarkable. First, all clusters, including C113, are characterized for having a single FeA ion located at the center of the cluster with the rest of ions in the surroundings giving rise to a cagelike structure. In the case of C33, this FeA ion is labeled as Ni = 5 关the corresponding in the bulk is FeA共2兲兴 in the cubic phase and as Ni = 2 关the corresponding in the bulk is FeA共1兲兴 in the monoclinic phase 共Tables IV and V兲. Such cation in the cluster exhibits a lost of charge accompanied by an increase in the magnetic moment relative to the corresponding atom in the bulk. Surprisingly, only in the C33F cluster, such central. FIG. 1. 共Color online兲 Optimized structures and valence electric charge distribution of the relaxed clusters originated from symmetry Fd3̄m corresponding to 共a兲 C33F, 共b兲 C45F, and 共c兲 C113F. Light gray 共yellow兲 small balls correspond to oxygens, black 共dark blue兲 for FeB ions 共and dark gray 共purple兲 in the case of C113F兲, whereas FeA ions are represented by light gray 共green兲 and 共gray兲 red spheres 共and a central black sphere in the case of C113F兲. Different colors correspond also to different charge and magnetization per atom values as described in Tables IV, VI, and VIII.. moment exhibits a parallel alignment respect to those spins of the B sublattice giving rise to a partial ferrimagnetic state different from the expected full ferrimagnetic behavior 共antiparallel alignment of the moments from the A and B sublattices兲. This scenario is the one responsible for the large value of the total magnetization observed for C33F. The interaction between the central atom with the rest is weak but non-negligible. For example, if the cohesive energy for that particular atom in the C33F cluster is calculated 共E33 − E32. TABLE IV. Valence electric charge and magnetic moment per atom for C33F. The units for charge and magnetization are e and B, respectively. Ni stands for the index employed in labeling the atoms within the cluster, whereas the corresponding positions in the bulk are indicated in parentheses. Ni. Atom. Qi. 1–4 5 6,7,10,13,16,17 8,11,14 9,12,15. FeA共1兲 FeA共2兲 Fe共B1兲 Fe共B2兲 Fe共B3兲. 1.99⫾ 0.04 0.38 −0.40⫾ 0.02 −0.39 −0.39⫾ 0.02. i −3.62 2.90 3.62 3.62 3.62. Color green red blue blue blue. FIG. 2. 共Color online兲 Optimized structures and valence electric charge distribution of the relaxed clusters originated from symmetry P2 / c corresponding to 共a兲 C33P, 共b兲 C45P, and 共c兲 C113P. Light gray 共yellow兲 small balls correspond to oxygens, black 共dark blue兲 for FeB ions, and gray 共light blue兲 for FeA ions.. 085107-4.
(5) PHYSICAL REVIEW B 80, 085107 共2009兲. STRUCTURE AND ELECTRONIC PROPERTIES OF IRON… TABLE V. Valence electric charge and magnetic moment per atom for C33P. The units of charge and magnetization are e and B, respectively. Ni stands for the index employed in labeling the atoms within the cluster, whereas the corresponding positions in the bulk are indicated in parentheses.. TABLE VII. Valence electric charge and magnetic moment per atom for C45P. The units of charge and magnetization are e and B, respectively. Ni stands for the index employed in labeling the atoms within the cluster, whereas the corresponding positions in the bulk are indicated in parentheses.. Ni. Atom. Qi. i. Ni. Atom. Qi. i. 1,4,5 2 3 6 9 10 7 8,12,15,16 11 13,14 17. FeA共3兲 FeA共1兲 FeA共3兲 FeB共9兲 FeB共9兲 FeB共9兲 FeB共11兲 FeB共12兲 FeB共11兲 FeB共10兲 FeB共10兲. 1.02⫾ 0.09 0.55 0.66 0.67 1.35 1.14 0.93 1.21⫾ 0.06 0.68 1.31⫾ 0.02 0.74. −3.62 −2.98 −3.62 3.63 3.63 3.63 3.63 3.63 3.63 3.62 3.62. 1 2 3,5 4 6,10 7 8 9 11 12 13,14 15 16 17. FeA共3兲 FeA共1兲 FeA共3兲 FeA共3兲 FeA共9兲 FeB共11兲 FeB共12兲 FeB共10兲 FeB共11兲 FeB共12兲 FeB共10兲 FeB共12兲 FeB共12兲 FeB共10兲. 1.20 1.61 1.32⫾ 0.05 0.37 1.71⫾ 0.06 0.94 1.75 1.21 1.32 1.86 1.77⫾ 0.05 1.68 1.59 1.85. −3.66 −3.84 −3.65 −3.66 3.45 3.43 4.13 4.12 4.13 3.43 3.47 3.46 3.50 3.50. − E1兲, a value of 1.67 eV is obtained, whereas a 6.74 eV value is obtained for the C45F cluster. Therefore, we can conclude that even though the central atom is bound to their neighbors, there is an electronic interaction between the central atom and the rest of the cluster. This fact can be also deduced from the spacial distribution of the electronic density curves shown in Fig. 3共a兲 as two-dimensional projections along different planes. The slight distortion in the density curves around the central atom due to the presence of its surroundings neighbors endorse the occurrence of such a weak interaction. The degree of distortion is greater for larger clusters 关e.g., C45P, Fig. 3共b兲兴. The rest of Fe cations, forming the cluster surface and representing the 97% of the total, are characterized by an increase in the electric charge relative to the corresponding atoms embedded in the bulk 共all the ⌬Qi, defined as Qi − Qbulk, are positive兲. The same conclusion is valid if the charge values are compared to those of the free atoms 共Qi − q兲. Results evidence therefore a charge transfer process between Fe and O cations. It must be stressed that despite the electric charge of oxygens atoms is not shown in the tables, the corresponding ⌬Qi were negative. Charge transfer is also observed for C45 and C113 clusters independently of what the starting symmetry was and. with a marked tendency of the surface Fe atoms to increase their electric charge. It can be concluded so far that a reordering of the charge and magnetic moment occurs as the system size decreases to nanoscale. We have also calculated the total DOS of the relaxed clusters and bulk magnetite. Zero energy was defined occurring at the Fermi level. Under bulk conditions and Fd3̄m symmetry, magnetite exhibits a metallic behavior 共⌬g = 0兲 with the Fermi level sitting in the middle of the spin-down Fe共B兲t2g band 共Fig. 4兲. Figure 5 shows the opening of an energy gap ⌬g at the Fermi level as the cubic structure is transformed. TABLE VI. Valence electric charge and magnetic moment per atom for C45F. The units of charge and magnetization are e and B, respectively. Ni stands for the index employed in labeling the atoms within the cluster, whereas the corresponding positions in the bulk are indicated in parentheses. Ni. Atom. 1–4 5 6,7,10,13,16,17 8,11,14 9,12,15. FeA共1兲 FeA共2兲 Fe共B1兲 Fe共B2兲 Fe共B3兲. i. Qi 1.47 2.03 1.61 1.61 1.61. −3.69 −3.84 3.71 3.71 3.71. Color green red blue blue blue. FIG. 3. 共Color online兲 Two-dimensional projections of the electronic density curves for 共a兲 C33F and 共b兲 C45P.. 085107-5.
(6) PHYSICAL REVIEW B 80, 085107 共2009兲. LÓPEZ et al. 300 200. 20. Density (states/eV). Density (states/eV). 30. 10 0 -10 -20. 100 0 -100 -200. -30 -3. -2. -1. 0. 1. 2. -300. 3. Energy (eV). -2. -1. 0. 1. 2. 3. Energy (eV). FIG. 4. 共Color online兲 Total electron DOS for the spin-up 共top兲 and spin-down 共bottom兲 electrons in bulk magnetite with cubic Fd3̄m symmetry. The Fermi level is at zero energy.. into the monoclinic structure. This gap 共0.25 eV兲, giving rise to an insulating state, is larger than the experimental value of 0.14 eV obtained by optical measurements at T = 10 K,31 but is close to the values obtained in other electronic structure calculations.14,15,30,37 As concerns to the clusters, it is evident the discrete character of the energy levels arising from two contributions, atomic electron levels, and bonding states coming from hybridized orbitals. Figures 6 and 7 show the total DOS of the relaxed C113 clusters for the two considered initial structures. Zero energy was defined occurring at the highest occupied molecular orbital. By comparing with those results under bulk conditions, the signature of a metallic behavior is still preserved for C113F, whereas in the case of C113P the width of the band gap in the minority spin channel increases to 0.3 eV reinforcing the onset of an insulating state. The scenario is more complex for smaller clusters, namely C33 and C45, where is difficult to identify a band gap due to the discrete character of the energy levels. Despite that, it is possible however to infer an energy gap whose size dependence is not monotonous according to the nonmonotonous Fe:O ratio in the studied clusters. In any case, the width of the gap in the minority spin channel for C33P and C45P clusters was estimated around 1 eV reinforcing even more the insulating state. Figure 8 shows the charge distribution for the C113F cluster. Results reveal a charge and magnetic moment reordering relative to the bulk. Such a reordering gives rise to an increase in the number of nonequivalent Fe atoms from four. FIG. 6. 共Color online兲 Total electron DOS for the spin-up 共top兲 and spin-down 共bottom兲 electrons for C113F clusters.. 共in the bulk兲 to six 共in the cluster兲, as can be deduced from Table VIII. Such a reordering scenario is characterized by the presence of Fe pairs on the surface having both the same charge 共1.80⫾ 0.03e兲 and the same magnetic moment per atom 共3.72B兲. The formation of such dimers, consistent with a charge-ordering scenario, has been already reported to occur in magnetite on the basis of the so-called bond dimerization model.15,38 Regarding the magnetic structure, the iron magnetic moments amount between −3.97B and 4.11B. Different from this, C33F and C45F clusters are characterized only by three nonequivalent iron atoms. The number of such nonequivalent Fe atoms increases dramatically for those clusters originated from P2 / c symmetry. In the case of C113P clusters, that number is as bigger as 30 indicating a high degree of disorder as concerns to charge and magnetic moment distribution. Variations in charge and magnetization, relative to the bulk, have also been analyzed as a function of the position of the atoms relative to the center of the cluster. The corresponding results for C33F are shown in Figs. 9 and 10. For this cluster size there is a clear tendency of the average charge to increase from the center to the surface. Contrary to this, the average magnetization decreases in the same direction and a linear relationship between the mean values 具⌬Q典 and 具⌬典 can be inferred. Analogously, a linear relationship is also obtained for C45F. Such a well-behaved dependence, holding only for the smallest clusters, is not longer observed for C113F where such quantities seem to be uncorrelated. This fact can presumably be ascribed to a higher degree of disorder due to the increase in nonequivalent iron sites hav-. 75. 150. 50. 100. 25. Density (states/eV). Density (states/eV). -3. 0 -25 -50 -75. 50 0 -50 -100. -3. -2. -1. 0. 1. 2. 3. -150. Energy (eV). FIG. 5. 共Color online兲 Total electron DOS for the spin-up 共top兲 and spin-down 共bottom兲 electrons in bulk magnetite with monoclinic P2 / c symmetry. The Fermi level is at zero energy.. -3. -2. -1. 0. 1. 2. 3. Energy (eV). FIG. 7. 共Color online兲 Total electron DOS for the spin-up 共top兲 and spin-down 共bottom兲 electrons for C113P clusters.. 085107-6.
(7) PHYSICAL REVIEW B 80, 085107 共2009兲. STRUCTURE AND ELECTRONIC PROPERTIES OF IRON… TABLE VIII. Valence electric charge and magnetic moment per atom for C113F. The units of charge and magnetization are e and B, respectively. Ni stands for the index employed in labeling the atoms within the cluster, whereas the corresponding positions in the bulk are indicated in parentheses. Ni. Atom. Qi. 1,3–9,11,13,16,17 2,10,12,14 15 18–20 24,28 35 45 21 25 32,42 39–41 22,23,27,33,43,44 26,34 29–31,36–38. FeA共2兲 FeA共1兲 FeA共2兲 Fe共B2兲 Fe共B2兲 Fe共B2兲 Fe共B2兲 Fe共B3兲 Fe共B3兲 Fe共B3兲 Fe共B3兲 Fe共B1兲 Fe共B1兲 Fe共B1兲. 1.29⫾ 0.04 1.62⫾ 0.01 1.64 1.79⫾ 0.01 1.54 1.37 1.39 1.38 1.37 1.52⫾ 0.01 1.80⫾ 0.03 1.45⫾ 0.08 1.38⫾ 0.01 1.80⫾ 0.03. i −3.96 −3.92 −3.97 3.72 4.11 4.11 3.58 3.58 4.11 4.11 3.72 4.11 3.58 3.72. Color red green black purple blue blue cyan cyan blue blue purple blue cyan purple. ing the same charge and concomitantly different values of the magnetic moment, which is not the case for smallest clusters. As concerns to the structural characterization of the clusters, both the radial and angular distribution functions were computed. In Figs. 11 and 12 such functions for C113P clusters before and after the relaxation process are displayed. In all cases the initial atomic positions used as input parameters were obtained from literature and they correspond to highresolution structural refinement analysis of our reference material.29 Due to the reduced number of atoms in these systems and the high degree of discreteness, each cluster represents a particular scenario with a particular structural signature resulting in different RDF and ADF functions. An important feature, common to all the clusters, independently of the initial space group, is the peaks broadening after relaxation which is more noticeable in monoclinic clusters. It must be stressed that the conditions and the step resolution 共1.3 Å兲 were kept fixed in all cases. Thus, the broadening of peaks, associated to disorder, which is less marked in clusters originated from cubic symmetry, agrees with the greater. FIG. 8. 共Color online兲 Valence electric charge distribution for C113F clusters. Two different views of the cluster are displayed. Every color stands for a given set of charge and magnetic moment. Dimers are those represented by purple color corresponding to 6.95e and 3.72B.. FIG. 9. 共Color online兲 Variation of electric charge per atom relative to the bulk with the atomic position measured from the center for C33F clusters. Numbers 1 and 2 along the x axis stand for first and second nearest neighbors, respectively.. amount of nonequivalent iron sites observed in clusters originated from monoclinic symmetry. Atomic displacements give rise also to a different distribution of angles and consequently to a peaks broadening in the ADF function. A remarkable feature is also the change in the cluster volume after relaxation. Volume was computed by considering a sphere of a radius equals to the distance, relative to the center, of the outermost atom. For C113P a volume expansion from around 1039 Å3 to 1051 Å3 is observed, whereas a volume reduction from around 1002 Å3 to 985 Å3 takes place for C113F. Another particular interesting feature is the presence of a single atom very close to the geometrical center of the cluster with the rest of the atoms in the surroundings. This fact is easily visualized in Fig. 13 showing the distribution of atoms with the distance to the geometrical center of the cluster. As can be observed, atoms are located in groups of concentric layers separated by spaces in between, forming an onionlike structure. The thickness of such layers, which in turn corresponds to the peaks broadening observed in the RDF and ADF functions, depends on the distance and the type of cluster. A special case is the smallest cluster C33 with a single atom in the center and the remain-. FIG. 10. 共Color online兲 Variation of the magnetization per atom relative to the bulk with the atomic position measured from the center for C33F clusters.. 085107-7.
(8) PHYSICAL REVIEW B 80, 085107 共2009兲. LÓPEZ et al.. FIG. 11. 共Color online兲 Radial distribution function for C113P, before and after relaxation.. ing distributed on the surface, which corresponds to 97% of the total of atoms. As the cluster size increases it turns out more difficult to realize what is exactly the surface 共Figs. 13 and 14兲. Figure 14 shows the histogram of the number of atoms and the mean coordination number 共Eq. 共1兲兲 with the distance to the center of the cluster for C113P. As is observed, the mean coordination number decreases in a well-behaved fashion, characterized by a linear decrease above 2 Å. The groups of data points are separated by spaces accordingly to the way as the atoms are distributed as a function of distance.. FIG. 13. Distribution of the number of atoms with the distance measured respect to the center of the cluster for C33P 共top panel兲 and C45P 共bottom panel兲.. A metallic behavior of bulk magnetite in the cubic phase is concluded, whereas the monoclinic phase with P2 / c symmetry is characterized by an insulating band gap 共⌬g = 0.25 eV兲 in agreement with experimental results linked to the Verwey transition. Results evidence that the ground-state cohesive energy is much smaller in the P2 / c phase than in the Fd3̄m phase, indicating that the low-temperature monoclinic phase of P2 / c symmetry is energetically more stable. Even for clusters, the ground-state phase is that originated from a P2 / c structure. This fact suggests that magnetite nanoparticles should, in principle, exhibit Verwey transition. The signature of metallic behavior is still preserved for. C113F clusters, resembling a nonstoichiometric magnetite according to its Fe:O proportion, whereas in the case of C113P clusters the width of the band gap in the minority spin channel increases to 0.3 eV reinforcing the onset of an insulating state. The scenario is more complex for smaller clusters as long as the bands are not longer observed and the discrete character of the energy levels becomes dominant. Our ground-state calculations reveal also a partial dimerization on the surface of C113F clusters and six nonequivalent iron sites. The situation is different for C113P clusters characterized by a higher number of nonequivalent Fe sites associated to structural disorder. For C33 clusters, independently of the initial structure, the central Fe cation exhibits a lost of charge accompanied by a remarkable increase in the mag-. FIG. 12. 共Color online兲 Angular distribution function for C113P, before and after relaxation.. FIG. 14. Distribution of the number of atoms and mean coordination as functions of the distance measured respect to the center of the C113P cluster.. IV. CONCLUSIONS. 085107-8.
(9) PHYSICAL REVIEW B 80, 085107 共2009兲. STRUCTURE AND ELECTRONIC PROPERTIES OF IRON…. netic moment. For C33F such central moment becomes parallel aligned to those moments of the B sublattice. This alignment is the one responsible for the large value of the magnetization observed for this cluster size and it is related to the weak interaction between the central ion and its surroundings neighbors. Results reveal also a charge transfer process between Fe and O cations characterized by an increase in the electric charge of Fe cations on the surface. Such a charge transfer is also observed in C45 and C113 clusters. Variations in charge and magnetization were also analyzed as a function of the position of the atoms relative to the center of the clusters. Finally, a structural analysis based on the computation of radial and angular distribution functions as well as on histograms, showing the way as the atoms are located within the clusters, was carried out. In particular, results reveal a peaks broadening in the distribution functions attributed to atomic displacements, respect to the input positions, forming an onionlike structure. Such disorder is however confined to occur in layers of different thickness and caging the central atom. This broadening, which is less. ACKNOWLEDGMENTS. This work was supported by COLCIENCIAS, FONDECYT Grant Nos. 1050066 and 7080111, Millenium Science Nucleus “Basic and applied magnetism” P06-022F, Sostenibilidad projects of the Solid State and the Microelectronic and Scientific Instrumentation Groups of the Universidad de Antioquia, CODI-UdeA project No. IN565CE and PROALMEX Mexico-Germany binational collaboration project. A.H.R. and S.L. were supported by CONACyT México under the Project Nos. J-59853-F, No. J-83247-F, and MICINN of Spain under grant No. MAT2007-65990C03-03. J.M.Z. is grateful to Universidad de Antioquia and Colciencias for giving support. We also acknowledge the computer time provided by Universidad Politécnica de Valencia as well as CNS, and Ipicyt, México.. Hohenberg and W. Kohn, Phys. Rev. 136, B864 共1964兲; W. Kohn and L. J. Sham, ibid. 140, A1133 共1965兲. 17 S. L. Dudarev, G. A. Botton, S. Y. Savrasov, C. J. Humphreys, and A. P. Sutton, Phys. Rev. B 57, 1505 共1998兲. 18 J. P. Perdew, J. A. Chevary, S. H. Vosko, K. A. Jackson, M. R. Pederson, D. J. Singh, and C. Fiolhais, Phys. Rev. B 46, 6671共1992兲; 48, 4978共1993兲. 19 P. E. Blöchl, Phys. Rev. B 50, 17953 共1994兲. 20 G. Kresse and D. Joubert, Phys. Rev. B 59, 1758 共1999兲. 21 G. Kresse and J. Hafner, Phys. Rev. B 47, 558 共1993兲; 48, 13115 共1993兲; 49, 14251 共1994兲; G. Kresse and J. Furthmüller, Comput. Mater. Sci. 6, 15 共1996兲; G. Kresse and J. Furthmüller, Phys. Rev. B 54, 11169 共1996兲. 22 V. I. Anisimov, I. S. Elfimov, N. Hamada, and K. Terakura, Phys. Rev. B 54, 4387 共1996兲. 23 V. N. Antonov, B. N. Harmon, V. P. Antropov, A. Ya. Perlov, and A. N. Yaresko, Phys. Rev. B 64, 134410 共2001兲. 24 V. N. Antonov, B. N. Harmon, and A. N. Yaresko, Phys. Rev. B 67, 024417 共2003兲. 25 V. I. Anisimov, J. Zaanen, and O. K. Andersen, Phys. Rev. B 44, 943 共1991兲. 26 G. Henkelman, A. Arnaldsson, and H. Jónsson, Comput. Mater. Sci. 36, 354 共2006兲. 27 H. J. Monkhorst and J. D. Pack, Phys. Rev. B 13, 5188 共1976兲. 28 M. Methfessel and A. T. Paxton, Phys. Rev. B 40, 3616 共1989兲. 29 J. P. Wright, J. P. Attfield, and P. G. Radaelli, Phys. Rev. Lett. 87, 266401 共2001兲; Phys. Rev. B 66, 214422 共2002兲. 30 R. Aragón, Phys. Rev. B 46, 5328 共1992兲. 31 S. K. Park, T. Ishikawa, and Y. Tokura, Phys. Rev. B 58, 3717 共1998兲. 32 I. Leonov, A. N. Yaresko, V. N. Antonov, M. A. Korotin, and V. I. Anisimov, Phys. Rev. Lett. 93, 146404 共2004兲. 33 I. Leonov, A. N. Yaresko, V. N. Antonov, and V. I. Anisimov, Phys. Rev. B 74, 165117 共2006兲. 34 Z. Szotek, W. M. Temmerman, A. Svane, L. Petit, G. M. Stocks, 16 P.. *firstname.lastname@example.org †email@example.com ‡. firstname.lastname@example.org. §email@example.com 储. marked in clusters originated from cubic symmetry, agrees with the greater amount of nonequivalent iron sites observed in clusters originated from monoclinic symmetry.. firstname.lastname@example.org 1 B. V. Reddy and S. N. Khanna, Phys. Rev. Lett. 93, 068301 共2004兲. 2 B. V. Reddy, F. Rasouli, M. R. Hajaligol, and S. N. Khanna, Chem. Phys. Lett. 384, 242 共2004兲. 3 H. Wu, S. R. Desai, and L.-S. Wang, J. Am. Chem. Soc. 118, 5296 共1996兲. 4 L.-S. Wang, H. Wu, and S. R. Desai, Phys. Rev. Lett. 76, 4853 共1996兲. 5 D. M. Cox, D. J. Trevor, R. L. Whetten, E. A. Rohlfing, and A. Kaldor, Phys. Rev. B 32, 7290 共1985兲. 6 R. L. Whetten, D. M. Cox, D. J. Trevor, and A. Kaldor, Phys. Rev. Lett. 54, 1494 共1985兲. 7 D. N. Shin, Y. Matsuda, and E. R. Bernstein, J. Chem. Phys. 120, 4150 共2004兲; 120, 4157 共2004兲. 8 N. O. Jones, B. V. Reddy, F. Rasouli, and S. N. Khanna, Phys. Rev. B 72, 165411 共2005兲. 9 Q. Sun, A. K. Kandalam, Q. Wang, P. Jena, Y. Kawazoe, and M. Marquez, Phys. Rev. B 73, 134409 共2006兲. 10 Q. Wang, Q. Sun, M. Sakurai, J. Z. Yu, B. L. Gu, K. Sumiyama, and Y. Kawazoe, Phys. Rev. B 59, 12672 共1999兲. 11 Jens Kortus and Mark R. Pederson, Phys. Rev. B 62, 5755 共2000兲. 12 Q. Sun, M. Sakurai, Q. Wang, J. Z. Yu, G. H. Wang, K. Sumiyama, and Y. Kawazoe, Phys. Rev. B 62, 8500 共2000兲. 13 L. Zhu, K. L. Yao, and Z. L. Liu, Phys. Rev. B 74, 035409 共2006兲. 14 P. Piekarz, Krzysztof Parlinski, and Andrzej M. Oleś, Phys. Rev. Lett. 97, 156402 共2006兲; Phys. Rev. B 76, 165124 共2007兲. 15 Horng-Tay Jeng, G. Y. Guo, and D. J. Huang, Phys. Rev. B 74, 195115 共2006兲; Phys. Rev. Lett. 93, 156403 共2004兲.. 085107-9.
(10) PHYSICAL REVIEW B 80, 085107 共2009兲. LÓPEZ et al. and H. Winter, Phys. Rev. B 68, 054415 共2003兲. Lodziana, Phys. Rev. Lett. 99, 206402 共2007兲. 36 N. Guigue-Millot, N. Keller, and P. Perriat, Phys. Rev. B 64, 012402 共2001兲. 35 Z.. 37. H. P. Pinto and S. D. Elliot, J. Phys.: Condens. Matter 18, 10427 共2006兲. 38 H. Seo, M. Ogata, and H. Fukuyama, Phys. Rev. B 65, 085107 共2002兲.. 085107-10.